Description

Description:

All materials on our website are shared by users. If you have any questions about copyright issues, please report us to resolve them. We are always happy to assist you.

Related Documents

Share

Transcript

applied sciences
Article
Cavity Design in Woodpile Based 3DPhotonic Crystals
Xu Zheng *, Mike P. C. Taverne *, Ying-Lung D. Ho *
ID
and John G. Rarity *
Department of Electrical and Electronic Engineering, University of Bristol, Bristol, BS8 1US, UK
*
Correspondence: X.Zheng@bristol.ac.uk (X.Z.); Mike.Taverne@bristol.ac.uk (M.P.C.T.);Daniel.Ho@bristol.ac.uk (Y.-L.D.H.); John.Rarity@bristol.ac.uk (J.G.R.)Received: 25 May 2018; Accepted: 3 July 2018; Published: 5 July 2018
Abstract:
In this paper, we present a design of a three-dimensional (3D) photonic crystal (PhC)nanocavity based on an optimized woodpile structure. By carefully choosing the position of the
defect at the lattice center, we can create a cavity with high symmetry which supports well conﬁnedGaussian-like cavity modes similar to those seen in a Fabry Perot laser resonator. We could also tune
the resonant frequency of the cavity and manually choose the cavity mode order by adjusting the size
of the defect at a chosen position.
Keywords:
3D photonic crystal; woodpile; photonic band gap; microcavity; cavity mode
1. Introduction
There has been signiﬁcant interest in three-dimensional photonic crystal (3D PhC) structures in
recent years aiming to exploit full photonic band gaps (PBG) [
1
–
3
] and the unprecedented conﬁnementof light at defects in these structures. A variety of structures have shown complete photonic bandgaps
including dielectric spheres in a face-centered-cubic (FCC) lattice [
4
–
6
], rod-connected diamond(RCD) structures [
7
,
8
], ‘Yablonovite’ PhC [
9
] and woodpile based PhC structure [
10
]. Variousdefects can be introduced in such perfect crystals to create localized photonic modes such as opticalwaveguides
[11–15]
and nanocavities [
16
–
22
]. Light trapped in such defects interacts strongly withlight emitters making them suitable for ultra-low-threshold lasers [
23
–
26
], enhanced optoelectronicsensors [
27
–
30
], ultrafast and low-power all-optical switches [
31
–
34
] and quantum informationprocessing devices with non-linearity at the single photon level [
35
–
38
]. Although much effort has
been made in applications of 1D or 2D PhCs [
39
–
42
], they still lose the conﬁnement of light in the third
dimension but rely on a total internal reﬂection. This leads to out-of-plane losses and manufactural
restrictions such as suspended membranes or low index substrates. In a 3D PhC structure, the cavity
mode is strongly associated with the surrounding environment which could result in a rich varietyof mode patterns. Recently, fabrication of 3D photonic structures by direct laser writing (DLW)using two-photon polymerization (TPP) [
43
] has been reported creating woodpile [
44
–
47
] and RCDstructures [
48
]. Notably, the woodpile structure is a promising structure which could be possibleto mass produce with lower cost methods via layer by layer 2D lithographic approaches [
13
,
49
].Although current applications are rather limited by the challenges of fabrications, some pioneeringwork has been proposed and implemented for various applications such as photon guiding [
13
,
49
]
and spontaneous-emission control [50].
In this study, we choose a woodpile structure formed by rectangular rods as the template. Design
of the defect in such woodpile based 3D PhC structures is investigated through comparing thewoodpile lattice with the RCD lattice [
8
]. Although a woodpile formed by rectangular rods may not
hold the widest photonic bandgap record as an inverse woodpile [
10
] or a RCD structure does [
6
–
8
],such discussion about the position of a defect based on the lattice still could apply more generally to
Appl. Sci.
2018
,
8
, 1087; doi:10.3390/app8071087 www.mdpi.com/journal/applsci
Appl. Sci.
2018
,
8
, 1087 2 of 11
other kinds of structures [
21
]. We found that, by carefully choosing the position of the defect, we could
create a cavity with high symmetry which supports well conﬁned cavity modes and also demonstratethat such a cavity in a woodpile based 3D PhC structure works in a similar way to a Fabry Perot laserresonator [
51
]. Moreover, choosing the speciﬁc defect position can help to simplify the analysis of themode pattern as a result of the combination of the cavity with and without the 3D PhC surroundings.
This paper is organized as follows. In Section 2, we introduce the simulation methods applied
throughout this paper. We then detail the designed woodpile structure in Section 3 with optimized
parametersusedinoursimulationsandthepositionwechooseforthecavity. Theprincipleofchoosing
this position is also discussed. In Section 4, we show the numerical results to demonstrate the tunable
cavity mode and mode volume.
2. Calculation Methods
We ﬁrst use the plane-wave expansion (PWE) method [
52
] to calculate the band structure for the
woodpile template without any defect in the frequency domain. This gives us the dispersion relation of
the woodpile template and the position of the complete photonic bandgap. We then use our in-house
three-dimensional ﬁnite-difference time-domain (FDTD) software [
17
,
20
,
21
,
53
] with perfectly-matchedlayer (PML) boundaryandanon-homogeneousmeshof around10
7
cells toimplement eachsimulation
when various defects are introduced into the woodpile template. A broadband dipole source andmultiple ﬁeld probes are placed inside the defect to excite and monitor the ﬁeld decay over time.The resonant frequencies f
c
, linewidths
∆
f and Q factors (deﬁned as f
c
/
∆
f) are then estimated byanalysing the ﬁeld decay in the frequency domain via the fast Fourier transform (FFT) and the ﬁlter
diagonalization method using the Harminv software [
54
]. Effective mode volumes are also calculated
using the deﬁnition,V
eff
=
ε
(
r
)|E(
r
)|
2
d
3
r/[
ε
(
r
)|E(
r
)|
2
]
max
, (1)
where E(
r
) is the resonant ﬁeld and
ε
(
r
) is the dielectric constant at position
r
. For each resonant
mode, we take the integration of the mode energy through sufﬁcient computational volume to ensure
convergence.
3. Woodpile Parameters and Cavity Design
In Figure 1a we show the woodpile structure we are modelling. The woodpile forms an FCClattice when the height of the rods
h
is equal to
c
/4 [
1
], and the distance between two adjacent rods
d
=
c
/
√
2 where
c
indicates the vertical period which is also the height of four stacking layers. Before
we show the numerical results and the defect design, we choose the optimized woodpile with widest
complete photonic bandgap simply by adjusting the width
w
of the rods [
20
]. Throughout this work
the refractive index of logs is
n
rod
= 3.3, corresponding to common semiconductor materials such asGallium Phosphide (GaP), while the background material is air
n
air
= 1. Figure 1 b shows the bandstructure calculated using plane-wave expansion (PWE) [
52
] method. The green region indicatesthe location of the optimized complete photonic bandgap which ranges from normalized frequency
c/
λ
= 0.485 to 0.569 (where
λ
is the wavelength) and the gap/midgap ratio reaches a maximum valueof 15.88% when the width of rods
w
= 0.21
c
[
20
]. All the simulations shown in this paper are based on
this woodpile template with optimized parameter speciﬁed in Figure 1.
Since we have the optimized woodpile, we start to introduce a rectangular parallelepiped defect
to create a cavity. The whole simulated woodpile template has 37 stacking layers in the z direction and
13 rods in each layer. The location of the defect is placed between the 19th layer and the 20th layer
counting from the bottom. The refractive index of the defect is the same as that of the rods
n
defect
= 3.3
in this paper. Figure 2 shows the location of the defect in one vertical period (four stacking layers in
z
axis). The defect is placed between the middle layers and the height of the defect is 2
h
which makes
it connect with both rods in the upper and lower layer. In both middle layers, the center of defect is
also between two adjacent rods.
Appl. Sci.
2018
,
8
, 1087 3 of 11
Figure 1.
(
a
) Parameters of the woodpile structure deﬁned in the simulation: vertical period
c
, height of rods
h
=
c
/4, distance between adjacent logs
d
=
c
/
√
2 and width of rods
w
. The refractive index of rods
is
n
rod
= 3.3, while the background material is air
n
air
= 1; (
b
) The calculated band structure by using
plane-waveexpansion(PWE)method[
52
]withoptimizedparameters. Thecompletephotonicbandgap
reaches a maximum value of 15.88% when
w
= 0.21
c
[
20
]. The insets illustrate the symmetric pointsin Brillouin zone of the face-centered-cubic (FCC) lattice relative to the woodpile and the calculation
routes to obtain the complete photonic bandgap.
Figure 2.
The location of the defect in one vertical period (four stacking layers in the
z
direction).
(
a
) view of the
xz
-plane (
b
) view of the
yz
-plane (
c
) view of the
xy
-plane (from the top) and (
d
) the free3D view.
L
is the size of the defect in
x
and
y
direction while the height is always 2
h
to make it connect
with both rods at the bottom and top.
Appl. Sci.
2018
,
8
, 1087 4 of 11
Woodpile is face-center-cubic (FCC) structure, which could be considered as a rod-connecteddiamond lattice. As shown in Figure 3, rods in different colors in rod-connected diamond lattice (a)
stand for different layers in woodpile lattice (b) [
8
]. The woodpile structure is obtained by substituting
short rods in rod-connected diamond lattice with a single long rod. The position of defects shown in
this paper is thus chosen from the body center of the lattice to get the most symmetrical position.
Figure 3.
The comparison between rod-connected diamond lattice (
a
) and woodpile lattice (
b
).
Woodpile could be considered as a layered version of the rod-connected diamond structure [8].
4. Numerical Results
In this section, we use the ﬁnite-difference time-domain (FDTD) method to simulate the cavitymode estimating the resonant mode frequency and Q-factor in various defects when changing thesize of the defect
L
from 0.1
c
–2
c
. A broadband dipole source whose bandwidth covers the complete
photonic bandgap is positioned at the center of the cavity and along the
z
-axis. We demonstrate that
effective mode volumes of the cavity mode could be suppressed by making the defect smaller, and
Q-factors of cavities can become high when the resonant frequency is located around the center of the
complete photonic bandgap. Figure 4 illustrates all the high Q-factor cavity modes we ﬁnd near and
inside the photonic bandgap as the defect size
L
is increased. The dashed lines indicate the boundary
of the complete photonic bandgap and the position of the bandgap center related to the woodpile
templatewithoutadefect. WeﬁndthathighQ-factorcavitymodesdonotexistfaroutsidethebandgap
as expected although some of them appear at the band edge. Furthermore, the normalized resonantfrequency of both fundamental modes (Mode 1) and high order modes (Mode 2–5) decreases when
increasing the defect size
L
. The calculated Q-factors for the fundamental modes (Mode 1, black square
in Figure 4) are shown in Figure 5 as a function of normalized resonant frequency when defect size
L
ranges from 0.1
c
–0.8
c
. The Q-factor reaches its maximum value near the middle of the photonic bandgap when defect size
L
= 0.25
c
. As we use a ﬁnite structure in our simulation, the reﬂectivity
drops when the frequency moves away from the bandgap center resulting in a drop of the Q-factor.
For those cavity modes inside the complete photonic bandgap when the defect size
0.15
c
≤
L
≤
0.6
c
, the calculated normalized mode volumes are shown along with the Q-factors inFigure 6. It is shown that the calculated normalized mode volume reduces from 0.64 to 0.29 (
λ
/
n
)
3
whenthedefectsize
L
decreasesfrom0.4
c
to0.15
c
,whileQ-factorreachesthehighestvalueof1.24
×
10
5
when
L
= 0.25
c
and starts to drop quickly if the defect size is further reduced. As the cavity mode
approaches the band edge the mode volume reaches a minimum because the ﬁeld outside the bandgapisnotconﬁned. For
L
>0.4
c
themodevolumeappearstodecreaseslightlywhichmaybeaconsequence
of limited calculation space when the mode approaches the band edge and becomes leaky. Figure 7illustrates the energy distribution of cavity modes when defect size
L
= 0.5
c
,
L
= 0.25
c
,
L
= 0.2
c
and
L
=0.15
c
,respectively. InFigure7,weobservenearlyperfectGaussianconﬁnementinsuchdefectswith
“wings” (predominantly blue areas) ﬂoating inside the adjacent dielectric rods. Furthermore, we see

We Need Your Support

Thank you for visiting our website and your interest in our free products and services. We are nonprofit website to share and download documents. To the running of this website, we need your help to support us.

Thanks to everyone for your continued support.

No, Thanks

SAVE OUR EARTH

We need your sign to support Project to invent "SMART AND CONTROLLABLE REFLECTIVE BALLOONS" to cover the Sun and Save Our Earth.

More details...Sign Now!

We are very appreciated for your Prompt Action!

x